technologies for mitigating these emissions, fuel cells have the
ability to efﬁciently convert chemical into electrical energy. In
particular, PEMFCs are zero-pollutants emission systems because
they transform the chemical energy of the electrochemical reac-
tion within hydrogen and oxygen into clean electrical power [1,2].
Generally, they work at To100 1C, making possible a rapid start-
up. Unfortunately, as a principal drawback, PEMFCs need to be
supplied by high purity hydrogen since the anodic Pt-based
catalyst tolerates less than 10 ppm of CO. The hydrogen is
industrially produced as a hydrogen-rich stream mainly via steam
reforming of natural gas in conventional reformers (CRs) .
Successively, hydrogen is puriﬁed to reach the desired purity for
the PEMFC supply. Indeed, the reformed stream coming out from
the CRs commonly contains hydrogen, CO2, CO, CH4 and other
byproducts. As a consequence, PEMFCs supply imposes the pur-
iﬁcation of hydrogen, which commonly takes place in second stage
processes, namely water gas shift (WGS) reaction (performed in
two reactors operating in series at high and low temperatures),
partial oxidation (PROX) and pressure swing adsorption (PSA)
[4–6]. Nevertheless, the aforementioned stages of hydrogen pur-
iﬁcation affect negatively the overall process in terms of costs and
efﬁciency . Hence, at scientiﬁc level much attention has gained
the development of alternative technologies to generate high
purity hydrogen (or, at least, COx-free) for PEMFCs supply. Among
them, membrane reactors (MRs) technology plays an important
role as an alternative solution to the conventional systems
(CRsþfurther stage of hydrogen puriﬁcation systems) in terms
of combination in a single stage of the reforming reaction for
generating hydrogen and its puriﬁcation without needing any
further process/treatment . As shown in Fig. 1, the interest
towards this technology is testiﬁed by the growing number of
scientiﬁc publications in the specialized literature.
As a particular aspect regarding membrane technology,
the inorganic MRs utilization makes possible several beneﬁts over
the CRs [10–12], although they also present some drawbacks as
summarized in Table 1.
In particular, in the last decades, an extensive literature has
been addressed to hydrogen production using inorganic MRs
based on both dense and supported Pd-based membranes [13–25],
because of their high perm-selectivity to hydrogen with respect to
all other gases.
Meanwhile, compared to other feedstocks, methanol exploita-
tion shows various advantages as a hydrogen carrier for fuel cell
applications and, namely, it can be produced from renewable
sources  and the reforming reaction occurs at relatively low
temperatures, ca. 240–260 1C , compared to the methane
reforming, normally performed at 800–1000 1C . Methanol
steam reforming (MSR) reaction has been seen as a very attractive
and promising process for hydrogen production and, according to
the scientiﬁc literature on the argument, it can be described by the
following chemical reactions:
CH3OHþH2O ¼ CO2 þ3H2 ΔH1298 K ¼ þ49:7 ðkJ=molÞ ð1Þ
COþH2O ¼ CO2 þH2 ΔH1298 K ¼ 41:2 ðkJ=molÞ ð2Þ
CH3OH ¼ COþ2H2 ΔH1298 K þ90:7 ðkJ=molÞ ð3Þ
Reaction (1), represents MSR reaction, reaction (2) represents
water gas shift reaction and reaction (3) represents the methanol
decomposition reaction. Only the WGS reaction is exothermic and
takes place without variation of moles number. The steam reform-
ing reaction besides being endothermic takes place with an
increase of moles number. Unfortunately, the main drawback of
this process is represented by the CO formation as a byproduct,
which – as stated previously – can poison the anodic catalyst of
the PEMFCs as well as affect negatively the permeation of Pd-
based MRs . Indeed, in the ﬁeld of MSR reaction performed in
CRs, several scientists paid special attention to catalyst optimisa-
tion in order to reduce the CO content [27–38].
The aim of this review is then oriented in describing the earlier
state-of-the-art about the use of inorganic MRs technology for
conducting the MSR reaction targeting the production of PEMFC
2. Methanol steam reforming catalyst
MSR has been widely studied and the most common catalysts
are based on copper, such as Cu/ZnO/Al2O3, working at ca. 240–
260 1C [27,39,40]. Copper-based catalysts are very active and low
cost, even though they originate a signiﬁcant concentration of
carbon monoxide, show low stability and pyrophoric nature. As an
example, Conant et al.  studied CuO/ZnO/Al2O3 catalyst stabi-
lity at 250 1C and concluded that, after 60 h of operation, methanol
Fig. 1. Number of scientiﬁc papers on H2 production by MR technology vs year.
Scopus database: www.scopus.com.
Some of the most signiﬁcative beneﬁts and drawbacks of MRs utilization.
MRs beneﬁts MRs drawbacks
Compact unit in combining both reaction and hydrogen puriﬁcation
with a consequent capital costs reduction
High costs and low mechanical resistance in case of
Conversion enhancement of equilibrium limited reactions. Higher
conversions than CRs (exercised at the same MRs conditions) or
at the same conversion of CRs reached at milder operating conditions
Not high purity hydrogen production in the case of
composite Pd-based MRs. Not high hydrogen perm-selectivity
in the case of non Pd-based MRs utilization
Direct production of high purity hydrogen in a single unit
(in the case of a dense Pd-based MR)
Hydrogen embrittlement at To300 1C in the case of dense Pd-MRs
Retentate stream of MRs rich in CO2 (i.e. the stream not permeated
through the membrane) when performing reforming reactions
Contamination of H2S, coke CO, etc. in the case of Pd-MRs
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368
conversion dropped 40%. Catalyst deactivation can be then caused
by sintering, coke deposition, catalyst poisoning (chloride, sul-
phur) and change in oxidation state. Coke formation can be
prevented using the water molar fraction above the stoichiometry
(Eq. (1)) and, generally, the best results are obtained for molar
water/methanol ratio of 1.5:1.
Therefore, the development of MSR catalysts more active,
stable and producing less carbon monoxide are needed. Especially,
catalysts that can operate at ca. 180 1C are strongly desired since
they are expected to be more stable and to produce less carbon
monoxide (Eq. (3) is disfavored for lower temperatures) and
thermodynamically they show almost complete conversion. More-
over, since MSR is an endothermic reaction, the reformer reactor
can be synergistically coupled with a high temperature (HT)-
PEMFC, which works exothermally. HT-PEMFC operates preferen-
tially in the range 160 1C and 180 1C. Despite the advantages of
working at 180 1C, copper based catalysts need activation that
occurs naturally when operating the reactor at temperatures
above 240 1C. For CuO/ZnO/Al2O3, this is carried out by reducing
the catalyst under hydrogen atmosphere at 250 1C.
Two approaches can be followed to prepare copper-based more
active catalysts and originating less carbon monoxide: (a) adding
promoters [42–45] and (b) changing the preparation method
[46,47]. Both approaches are used to increase the metal dispersion
and surface area and to decrease the particle size. The most used
promoters for copper-based catalysts are ZnO , ZrO2 , Mn
, CeO2  or Al2O3 . Furthermore, some materials can
affect the CO selectivity such as ZrO2  or change the surface
area where copper is dispersed such as alumina or chromium(III)
oxide . The catalyst preparation method is the second tool
available for improving the catalytic activity and the most used for
cooper-based catalysts are derivations from co-precipitation and
wet-impregnation. Depending on the promoters or the supports,
the more active catalyst of a speciﬁc type can be obtained by one
or other method or even by a derivation of the previous (e.g. to
produce CuZrO2 the best method is a derivation from co-
precipitation [53–55]). Alumina is one of the most used catalyst
support, but there are others such as carbon nanotubes that are
being investigated with promising results . Furthermore, other
interesting results were presented by Gao et al.  using a
Besides cooper-based catalysts, others are being studied for MSR
reaction, in particular those containing group VIII–X metals and,
especially, palladium. Pd/ZnO/Al2O3 catalyst presents higher stability
than Cu/ZnO/Al2O3 with an initial deactivation of 17%, afterwards
stable for 60 h . Pd/ZnO catalyst when compared with other
metals (Ni, Pt, Ru, Ir) supported on ZnO, presents lower CO produc-
tion and a higher methanol conversion [58–61]. The application of a
second metal to form bimetallic alloy can also improve the catalyst
activity and selectivity. The best activity reported was obtained with
Pd/Zn and Pd/Ga and the best selectivity with Pd/Cd . Pd catalysts
are drawing the attention of many researchers that are investigating
the role of the preparation methods , the effect of support surface
area  and the particle size . The search for more active and
selective catalysts for MSR resulted in a large number of articles that
were recently reviewed .
3. Methanol steam reforming reactors
The reactor design has direct impact on the reaction conver-
sion, but owing to higher technical complexity and manufacturing
costs of other designs, the reformers and MRs are normally
tubular. However, recent efforts in the area of micro-processing
made possible and easier to manufacture other reactor designs
and namely well-structured ﬂat micro-reactors. A micro-reactor is
deﬁned as a device that contains micro structured features, with a
sub-millimeter dimension, in which chemical reactions are per-
formed in a continuous manner . They present advantages
compared to conventional ones such as higher surface-to-volume
ratio, smaller mean distance of the speciﬁc ﬂuid volume to the
reactor walls, better heat and matter transfer properties and ﬂow
patterns that ﬁt with the reaction needs. Furthermore, ﬂat refor-
mers are suitable for stack integration with fuel cells.
Packed-bed micro-reactors require well-deﬁne catalyst parti-
cles, with regular shape and much smaller than the internal
dimensions of the micro-channels, which is a problem for most
of commercial catalysts  and, then, most of micro-reactors use
the catalyst applied as a coat. Micro-reactors range in area from
0.1 to 10 cm2
 and mini-reactors range between 10 and
. Mini-reactors, however, are more suitable for packed
bed applications and match the typical size of fuel cells.
MSR originates a stream that contains besides hydrogen, small
amounts of reactants, carbon dioxide and carbon monoxide. The
reformate stream needs, then, to be puriﬁed and dense Pd-
membrane reactors not only allow obtaining a high purity hydro-
gen stream but also contribute for improving the reformer con-
version. Pd-membrane reactors are normally tubular, even though
they can also be produced ﬂat [22,67].
Many studies have been developed to explore the advantages
of micro/mini-reactors to produce hydrogen through MSR. The
design of a reactor targets the maximization of the conversion and
selectivity at the lowest costs and its performance is inﬂuenced by
the ﬂow pattern, velocity proﬁle, pressure drop and heat transfer,
so all these aspects must be considered . For conducting MSR
reaction, most of the used reactor designs are rectilinear channels,
pin-hole, coil-based and radial (Fig. 2).
Coil-based reactor designs allow high conversions, but impose
a signiﬁcant pressure drop penalty, which may be a limitation
for compact applications . In the other hand, the rectilinear
channel designs exhibit a small-pressure drop, but the conversion
is low due to uneven mass distribution and is affected by the
Reynolds number . Yet, by adjusting the channels width 
or by imposing a pressure drop at the channels entrance even
distributions on rectilinear channel designs can be obtained,
improving the methanol conversion . The pinhole design has
Fig. 2. Different ﬂow ﬁeld designs of CRs. (a) coiled-serpentine; (b) Parallel multichannel; (c) Pin-hole; (d) Radial.
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368 357
great potential for innovative applications; it presents a methanol
conversion comparable to the coil reactor with lower pressure
drop. This design, however, exhibits a mass distribution that
depends on the Reynolds number. The ﬂow ﬁeld design should
provide even a distribution, independently of the Reynolds num-
ber, since the reactor is operated at different ﬂow rates.
Typically, the molar ﬂow rate of reformate streams is almost
twice the feed ﬂow rate, originating a signiﬁcant surface velocity
increase as the reaction stream moves along a constant cross
sectional area reactor. Moreover, since the pressure decreases
towards the exit of the reactor, the surface velocity increases even
more  (Fig. 3). For a diffusion-limited or close to diffusion-
limited reaction, this large variation of surface velocity can be very
detrimental for the conversion .
The radial reactor design, Fig. 2d, has unique features for MSR
because of the increase of section area as the gas moves to the
outlet, leading to low pressure drop compared to tubular reactor
and a close to constant velocity proﬁle (Fig. 3). Radial reactor
designs despite of the complex manufacturing originate higher
methanol conversions than channel designs .
The reactor design must minimize temperature gradients,
operating as close as possible of isothermal conditions. For channel
reactors, assuming only inter-particle temperature gradients, iso-
thermal conditions can be achieved by diminishing the channel
width [72,73]. However, the width of the channels should be ca.
300 μm in the case of MSR to avoid temperature gradients ,
which is not feasible for packed bed reactors, due to high-pressure
drop originated by the small particle size of the catalyst.
To minimize temperature gradients some strategies have been
considered such as internal heating  or wall coated reformers
[75–80]. Wall-coated reformers compared to packed-bed show low-
pressure drop and high heat transfer providing isothermal condi-
tions, but they have lower speciﬁc catalyst load. Nevertheless,
regarding the conversion and for a given contact time (W/F), some
studies indicate that wall-coated reformers better perform [72,78,79],
while others indicate similar performances . These different
conclusions might be related to differences in catalyst-layer packing
or coating methods, catalyst weight, channel width and operating
conditions . Inside the catalyst layer, heat transfer is dominated
by heat conduction (e.g. λCuO=ZnO=Al2O3
¼0.17 W m1
using glass beads or other inert particles with higher heat conduc-
tivity should improve the temperature distribution.
4. Outlook on membrane reactor technology and fuel cells
4.1. Membrane reactors
The comprehensive concept of MRs was introduced in the 1950s,
even if only with the exploitation of new inorganic materials and
the development of high-temperature membrane processes there
has been a growing interest towards the research and application
of MR technology . In fact, this is testiﬁed by an extensive
literature on MRs concerning different applications and scientiﬁc
ﬁelds. In detail, during the last 30 years different kind of MRs have
been developed and, as a general subdivision, they are summarized
in the following:
(a) Dense and porous inorganic membrane reactors [83,84].
(b) Zeolite membrane reactors [85,86].
(c) Polymeric membrane reactors [87,88].
(d) Enzyme membrane reactors 
(e) Bio-medical membrane reactors or membrane bio-reactors
using cells [90,91].
(f) Electrochemical membrane reactors (fuel cells, electrolytic
cells, etc.) .
(g) Photo-catalytic membrane reactors .
Recently, many scientists have proposed the application of
membranes combined to chemical and biochemical reactions in
order to intensify the whole process. Most of the approaches may
be classiﬁed concerning the role of membranes towards the
removal/addition of the various chemical species as: (a) extractor,
(b) distributor and (c) contactor. Membranes are generally cate-
gorized by referring to materials or structures, giving particular
relevance to the selectivity of the permeation of such a product
Fig. 3. (a) Pressure proﬁle in micro-channel reactor—ﬂuid pressure (atm) vs. distance (m); (b) velocity proﬁle in micro-channel reactor—ﬂuid velocity (m/s) vs. distance (m);
(c) Pressure proﬁle in radial reactor—ﬂuid pressure (atm) vs. distance (m); (d) velocity proﬁle in radial reactor—ﬂuid velocity (m/s) vs. distance (m), (adapted from ).
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368
with respect to other ones. However, in this review our attention is
devoted to the discussion on dense and porous inorganic mem-
brane reactors, able to integrate a chemical reaction (such as MSR)
with a membrane process (H2 separation). Commonly, the role of
the membrane in a membrane reactor can be described as:
Extractor, when it selectively removes the desired products
from the reaction mixture for permeation.
Distributor, when it controls the addition of reactants to the
Contactor, when it intensiﬁes the contact within reactants and
When a MR is performed in “extractor” mode, a desired
product obtained by the chemical reaction is selectively removed
from the reaction side for permeation through the membrane.
In the case of thermodynamic limited reactions, Extractor mode
can also be used to increase the selectivity towards a particular
intermediate species in a cascade reaction, if this species is
selectively removed from the reaction medium. Furthermore,
besides the beneﬁt of the shift effect, the extractor modality
may reduce sequential reactions. In particular, when the reaction
rate of the undesired secondary reactions is higher than that of
the main reaction, the reaction selectivity can be signiﬁcantly
increased by removing the desired intermediate species. Extrac-
tors have great application on dehydrogenations or reactions for
hydrogen production such as steam reforming or WGS, performed
using hydrogen selective membranes .
“Distributor” mode concerns the membrane utilization to add
uniformly a limiting reactant along the reactor space to prevent
hot spots and side reactions. For example, in partial oxidation
reactions, the membrane is used for selectively dosing oxygen
targeting both high conversions and product selectivities [95,96].
As a further beneﬁt, considering that the reactants and oxygen are
not premixed, mixtures are consequently avoided and ﬂame back
ﬁring into the feed is prevented.
MRs used in “contactor” mode make possible that the two-
sided geometry of the membranes may allow for different options
to bring reactants into contact.
4.2. Palladium-based MRs
Among the inorganic membranes, special attention should be
paid to dense palladium-based membranes owing to their full
hydrogen perm-selectivity. Nevertheless, between 0 and 700 1C
other metals such as niobium, vanadium and tantalum show
higher hydrogen permeability than palladium, even if they have
a stronger surface resistance to hydrogen transport than palla-
dium. Therefore, dense palladium membranes are greatly consid-
ered, although their commercialization is limited by some
drawbacks such as low hydrogen permeability and high costs
. The hydrogen molecular transport in palladium membranes
takes place through a solution/diffusion mechanism, developed in
six different activated steps: (a) dissociation of molecular hydro-
gen at the gas/metal interface; (b) adsorption of the atomic
hydrogen on membrane surface; (c) dissolution of atomic hydrogen
into the palladium matrix; (d) diffusion of atomic hydrogen through
the membrane; (e) re-combination of atomic hydrogen to form
hydrogen molecules at the gas/metal interface; (f) desorption of
hydrogen molecules. Generally, the hydrogen ﬂux permeating
through a generic membrane may be expressed as in the following:
is the hydrogen ﬂux permeating through the mem-
the hydrogen permeability, δ the membrane thickness,
pH2retentate and pH2permeate the hydrogen partial pressures in the
retentate (reaction side) and permeate (side in which hydrogen
permeating through the membrane is collected) zones, respec-
tively, n (variable in the range 0.5–1) the dependence factor of the
hydrogen ﬂux on the hydrogen partial pressure. For membranes
with thickness higher than 5 μm, Eq. (4) becomes the Sieverts–Fick
JH2;SievertsFick ¼ PeH2
For high pressures the hydrogen-hydrogen interactions in the
palladium bulk are not negligible, thus n becomes equal to 1:
Furthermore, if the hydrogen permeability is expressed as an
Arrhenius-like equation, Sieverts–Fick law becomes the Richard-
son′s Eq. (7):
when dense Pd-based membranes are exposed to pure hydrogen
permeation below both 300 1C and 2.0 MPa, the so called “hydro-
gen embrittlement” phenomenon may take place. It may be solved
by alloying palladium with other metals, such as silver, which
displays its electron donating behaviour, being largely similar to
that of the hydrogen atom in palladium, making possible competi-
tion for the ﬁlling of electron holes within the silver and hydrogen.
In MRs, the presence of hydrogen sulﬁde, SO2, Hg vapour,
thiophene, arsenic, unsaturated hydrocarbons, or chlorine carbon
from organic materials, etc. may contaminate dense Pd-based
membranes causing their irreversible poisoning . Furthermore,
the presence of CO in a MR affects negatively the hydrogen
permeation performances of the membrane, because the adsorbed
CO displaces the adsorbed hydrogen, blocking the hydrogen
adsorption sites. This effect is more intense at lower temperature
(below 150 1C) or at higher CO feed concentration [98,99]. Also
steam may poison dense Pd-based membranes by affecting the
water vapour dissociation/recombinative desorption, which con-
taminates the palladium surface with adsorbed oxygen .
During the last years, special attention has been devoted to
composite Pd-based MRs in order to reduce the amount of
palladium and consequently lowering the cost. Composite mem-
branes are constituted by a thin dense layer of palladium or its
alloy deposited onto porous supports such as porous Vycor glass
(silica gel), SiO2, Al2O3, and B2O3 or porous stainless steel (PSS).
The supports having a thermal expansion coefﬁcient close to the
palladium allow high mechanical durability and simplify the gas
sealing . Nevertheless, PSS support alloys the palladium at
relatively high temperatures, leading to lower the hydrogen
4.3. Proton exchange membrane fuel cells
PEMFCs gained a considerable attention because they represent
an alternative technology to produce green power due to the
chemical energy conversion of a fuel such as hydrogen directly
into electrical energy . Indeed, PEMFCs could represent a
viable solution to these issues because they are able to limit CO2
and other harmful emissions in the atmosphere. Unfortunately,
PEMFCs show also some drawbacks to enter fully in the market
such as the high cost of the membrane, fuel crossover, anodic
catalyst poisoning mainly caused by the CO and so on. PEMFCs are
commonly exercised at To100 1C and ambient pressure using
commercial membranes based on Naﬁon (produced by DuPont) as
a sulfonated perﬂuorinated polymer. Naﬁon shows great perfor-
mances in terms of proton conductivity and high potential at low-
medium temperature (up to 80–100 1C) and under fully hydrated
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368 359
conditions, whereas high costs, fuel crossover, loss of perfor-
mances at T4100 1C are the main Naﬁon drawbacks .
PEMFCs are fueled by pure hydrogen and the CO tolerance for
Tr80 1C is of a few ppm. As a consequence, much scientiﬁc
attention has been devoted to improve the catalyst tolerance to
CO, pointing out that Pt/Ru alloys are the most promising .
However, in the ﬁeld of high-temperature (HT) PEMFCs, Naﬁon
does not offer the best performances due to the reduced hydration
conditions. Therefore, other kinds of polymers are useful as
polymer electrolyte membranes instead of Naﬁon. Among them,
hybrid polymeric membranes based on blend of, for example,
sulfonated poly-ether-ether-ketone (S-PEEK) and poly-benzimida-
zole (PBI) or S-PEEK derivative membranes such as sulfonated
poly-ether-ether-ketone with cardo group (S-PEEK-WC) offer good
performances in terms of proton conductivity and resistance to fuel
crossover in the temperature range of 80–200 1C . Furthermore,
in the ﬁeld of HT-PEMFCs, CO tolerance of the anodic catalyst is
higher, around 20,000–30,000 ppm  and hydrogen does not
need to be highly puriﬁed, reducing the processes (and consequent
costs) useful for the hydrogen separation/puriﬁcation.
5. Feasibility study of methanol steam reforming reaction via
As reported in Fig. 4, the number of publications on ISI journals
regarding MSR reaction as a main topic is depicted during the
years, whereas the number of publications about the combination
between MSR reaction and MRs is shown in Fig. 5. It is quite
evident that, in both ﬁgures, the interest towards this kind of
reaction is grown even though membrane-based methanol
reforming systems have been studied by a number of academic
and industrial organizations only as a particular ﬁeld of a general
interest on MSR reaction .
However, MRs offer various beneﬁts over low-pressure systems
for hydrogen production combined with catalytic CO mitigation
even though they also show various drawbacks, particularly the
fragile nature of thin metal foils and the high cost.
MSR in MRs
Fig. 5. Number of publications on ISI journals vs years about MSR reaction in MRs
(Scopus database: www.scopus.com).
Some of the most representative experimental results about MSR reaction in MRs from the open literature.
Pd–Ag (3.9 mm layer)/
ELP Inﬁnite CuO/ZnO/Al2O3 1/1 600a
250 3 100 45 E100 
Pd–Ag (20–25 mm layer)/PSS ELP – CuO/ZnO/Al2O3 1.2/1 5b
240 10 36,1 18 – 
Carbon molecular sieve Pyrolysis 62c
CuO/ZnO/Al2O3 4/1 – 200 1 E95 E84 – 
SiO2/g-Al2O3/Pt-SiO2/PSS Soaking-rolling – Cu–Zn/based 1.3/1 – 230 – 100 9.1 – 
Pd (20 mm layer)/PSS ELP 4000 Cu/ZnO/Al2O3 1.2/1 10b
350 6 E95 97 99.9 
Pd–Ag/TiO2-Al2O3 ELP – Ru–Al2O3 4.5/1 – 550 1.3 65 – E72 
SiO2/g–Al2O3 Soaking-rolling E37 Cu-Zn/based 3/1 – 260 – 42 5 98 
Carbon-supported Pyrolysis E5.5 CuO/Al2O3/
3/1 – 250 2 55 – E80 
Carbon-supported – – Cu/ZnO/Al2O3 1.5/1 1b
250 2 E99 – 97 
Pd (20–25 mm layer)/PSS ELP Inﬁnite Cu-based 1.2/1 – 350 – 99 – E100 
Dense Pd–Ag (50 mm
Cold-rolling Inﬁnite CuO/Al2O3/
3/1 E0.4 300 3 – 80 E100 
Dense Pd–Ru–In (200 mm
– Inﬁnite Cu/ZnO/Al2O3 1.2/1 – 200 7 E90 E24 E100 
Dense Pd–Cu (25 mm
– Inﬁnite Cu–Zn based – – 300 10 4 90 E38 E100 
Fig. 4. Number of publications on ISI journals vs years about MSR reaction (Scopus
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368
In particular, the cost of palladium represents a potential barrier
for membrane-based systems to enter in the market. Therefore,
being the palladium intrinsically expensive, there has been in the
last years a crucial need to operate in MRs with thin supported
palladium membranes instead of dense self-supported foils and
much progress has been made in this area. Nowadays, most of the
methanol reforming units have been represented by MRs, mainly
for the advantageous reasons listed above and in spite of their
higher cost. In Table 2, the most representative results in terms of
conversion, hydrogen recovery and so on are reported about MSR
reaction performed in MRs. In detail, this table summarizes the
different typology of membranes used in MRs for conducting MSR
reaction besides the type of catalyst used and other important
parameters such as: H2/N2 ideal selectivity, H2O/MeOH feed ratio,
reaction pressure, reaction temperature, etc.
In particular, Table 2 points out that in the last years many
efforts have been made towards the development of composite
Pd-based membranes (a dense layer of Pd deposited onto a porous
support) and not Pd-based MSR membrane-based systems. Never-
theless, some data from literature are also given about the
utilization of dense, self-supported Pd-based membranes in order
to offer a more complete view on the topic. This table shows how,
by reducing the amount of palladium (in membranes constituted
by few microns of palladium layer deposited on porous supports),
in some case  it is possible to maintain the full H2/other gas
selectivity like the dense one [114,115] with high performances in
terms of methanol conversion and hydrogen recovery. However,
this table reports the most recent ﬁndings in this area referring to
composite Pd-based MRs for performing MSR reaction. More in
detail, one of the most signiﬁcant developments in the area is
represented by the study of Israni and Harold , who synthe-
sized a thin Pd–Ag layer (3.9 μm) deposited via electroless plating
deposition (ELP) onto a porous α-Al2O3 support. This membrane
shows a full H2/N2 perm-selectivity and allows to reach complete
methanol conversion during MSR reaction at 250 1C with a
hydrogen recovery varying from 45 to 95%, depending on the
reaction pressure in the range of 3–10 bar. In this case, the purity
of the hydrogen permeated stream was 100%. Also Lin and Rei
 prepared a supported Pd layer (20 μm) onto a porous
stainless steel (PSS) support with a H2/N2 perm-selectivity of
around 4000, useful for obtaining 95% of methanol conversion
with a hydrogen recovery of around 97% and a hydrogen permeate
purity of 99.9% at 6 bar and 350 1C. In other cases, the Pd-based
composite membranes did not give great results, probably because
the presence of defects in the Pd-layer affected the H2 perm-
selectivity with respect to all the other gases with a consequent
loss of performances in terms of conversion (due to a lower “shift
effect”), hydrogen recovery and purity. Table 2 also shows new
ﬁndings on not Pd-based MRs, namely carbon and silica-based
membranes [107,108,111–113]. In the study of Mendes and co-
workers , the carbon membrane from Carbon Membranes Ltd.
is developed via pyrolysis method of dense cellulose cupra-amonia
hollow ﬁbres and possesses relatively low H2/N2 perm-selectivity,
even if it allows to reach methanol conversion higher than 90%
with a hydrogen recovery480%. On the contrary, Briceño et al.
 prepared the supported carbon membrane based on a porous
ceramic support of TiO2 coated with ZrO2, onto which various
polymeric solutions as carbon precursors have been deposited
and, then, pyrolysed. The supported carbon membrane was useful
for obtaining a conversion higher than 50% and a hydrogen
permeate purity of around 80% .
In the same ﬁeld, Zhang et al.  used a carbon-based MR to
carry out MSR reaction. The carbon membrane was used as a
6-mm i.d. tube with a wall thickness of 20–3 μm and sealed inside
a stainless steel tube. As expected, methanol conversion equal to
almost 100% was reached in the carbon-based MR and it resulted,
as expected, higher than the conventional ﬁxed-bed reactor in the
temperature range of 200–250 1C. Furthermore, the hydrogen
permeate purity was found around 97%.
Lee′s group [108,111] used both supported SiO2/γ-Al2O3/Pt-
SiO2/PSS and SiO2/γ-Al2O3 membranes achieving different results
depending on the kind of membrane used in the MR. The ﬁrst
membrane was useful for achieving complete methanol conver-
sion even though the hydrogen recovery was quite low (o10%).
On the contrary, during the MSR reaction the second membrane
was able to give in the MR more than 40% of methanol conversion,
a poor hydrogen recovery but a quite interesting hydrogen purity
in the permeate (98%).
The reported experimental data in Table 2 about the application
of dense self-supported Pd-based membranes [114,115] show great
results in terms of complete conversion, high hydrogen recovery and
almost 100% hydrogen permeate purity, even if in these studies the
issue about the need of decreasing the palladium thickness is not
discussed. In particular, Basile′s group spent much attention in the
last years to carry out MSR reaction in inorganic MRs [110,114,120–
123]. They compared MRs and conventional ﬁxed-bed reactors by
investigating such parameters as reaction temperature and pressure,
time factor (residence time), H2O/MeOH feed molar ratio, sweep gas
ﬂow rate and its modality conﬁguration (co-current and counter-
current) with respect to the feed and oxygen addition (in the
oxidative MSR reaction ). Various membranes, both dense and
composite, in tubular and sheet shape, have been used during the
experimental tests of Basile and co-workers such as tubular dense
self-supported Pd77–Ag23 with a thickness of 50 μm produced at
ENEA Laboratory (Italy), dense Pd80–Ag20 sheet with a thickness of
60 μm produced at Laboratory of Noble Metals of Institute of
Metallurgy (RAS), tubular composite Pd–Ag/TiO2–Al2O3 produced at
CNR-ICCOM Laboratory (Italy), tubular composite Pd–Ag on asym-
metric ceramic support produced at University of Genova Laboratory
(Italy) and silica membranes from Department of Chemical Engineer-
ing, Nanostructure Material Research Center, Sahand University of
Technology, Tabriz (Iran). At any given condition, Basile and co-
workers demonstrated that the MRs show superior performances to
the CRs, operating at the same experimental conditions in terms of
methanol conversion, selectivity and productivity, all of which are
driven by the constant removal of hydrogen from the reactor zone.
However, other interesting studies are present in the open
literature and they are related to the need of new ﬁndings,
particularly oriented to prepare and use supported Pd-based
membranes to carry out MSR reaction. For example, Lin′s group
 used supported PSS Pd-membranes supplied by Worcester
Polytechnic Institute, in which the Pd-layer (20–25 μm) was
electroplated onto the support. They performed MSR reaction at
350 1C and with a H2O/MeOH feed ratio of 1.2/1, using a Cu-based
catalyst reaching conversion higher than 99% and with a pure
hydrogen recovery in the permeate side. Lin et al. theorized that a
reverse spillover mechanism is responsible for the improved
reaction rates obtained in Pd membrane reactors containing Cu-
based catalysts. Practically, they supposed that the formed hydro-
gen from the reforming reaction is able to migrate directly from
the active Cu-based catalyst site to the Pd membrane surface.
Han et al.  prepared a dense self-supported Pd–Cu mem-
brane with 25 μm thickness in order to carry out MSR reaction and
supply a 3-kW PEMFC. Complete conversion and hydrogen recov-
ery with a purity of 99.9999% are the main performances of this
MR. Successively, Han et al. [118,119] used a new generation of this
kind of MRs for a nominal 25-kW unit operating at 70–75%
recovery. The device was planned to be used in a PEM stack
(Hyundai Motors) and to integrate it a hybrid vehicle.
Other important researchers like Wieland et al.  carried out
MSR reaction in MRs by studying three different dense and self-
supported Pd-alloy membranes, Pd–Ag, Pd–Cu and Pd–V–Pd.
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368 361
Among them, Wieland′s group demonstrated that Pd–V–Pd mem-
brane (40 μm as a thickness) possesses high permeation rates, but
it is not stable and suffers mechanical cracks at pressure higher
than 6 bar. Pd–Cu membrane (25 μm as a thickness) was found
to be much more stable, but with lower hydrogen permeation
with respect to the third Pd–Ag membrane (40 μm of thickness).
Furthermore, they pointed out that the presence of CO or metha-
nol may signiﬁcantly affect the hydrogen permeating ﬂux through
the membrane because these components compete with the
adsorption of hydrogen, decreasing its permeating ﬂux by up to
70%. However, Wieland′s group found that, by using MRs housing
Pd–Cu and Pd–Ag membranes for the MSR reaction, at T¼300 1C
the conversion is higher than 99% at pressures higher than 5 bar
and it overcomes the equilibrium conversion of a correspondent
conventional reactor at pressures420 bar.
Furthermore, Fig. 6 shows a comparison in terms of methanol
conversion versus reaction temperature among the last 5 years
literature data for MSR performed in both CRs and MRs.
A direct comparison among all the experimental data from
literature reported in this ﬁgure is not possible owing to the different
operating conditions adopted by each author. Nevertheless, from a
qualitative point of view it is possible to observe that most of the
methanol conversions from the reported data about MRs is concen-
trated between 200 and 300 1C and their values are not lower than
50%. On the contrary, most of the methanol conversions from CRs
higher than 50% are reported in the temperature range from 300 to
400 1C. This aspect depicts to the reader a scenario in which great
methanol conversions are achievable from both CRs and MRs.
Nevertheless, MRs operate at lower reaction temperature than CRs
with a consequent possible beneﬁt in terms of energy saving.
Furthermore, as another beneﬁt MRs may collect a puriﬁed hydrogen
stream in the permeate side with a concentration depending on
which kind of membrane is utilized. Furthermore, another important
issue is represented by the concentration of CO in the hydrogen rich-
stream produced via MSR reaction for PEMFCs supply. As stated in
the ﬁrst part of this review, the CO concentration tolerance of such a
PEMFC depends on its operating temperature. In Table 3, some recent
experimental results from literature concerning CO concentration
in the MSR reformed stream of CRs [103,131,134–137] and both
permeate and retentate streams of MRs are shown. As well known,
low-temperature (LT)-PEMFCs work at To100 1C (commonlyE
80 1C) and the CO tolerance for the supplied hydrogen stream is
Literature data about CO level in the reformed stream of some CRs and in both permeate and retentate streams of some MRs.
T [1C] p [bar] Catalyst Membrane CO level in the
permeate side [ppm]
CO level in the
retentate side [ppm]
230 – Pt/SiO2–Cu/Zn SiO2/g-Al2O3/Pt-SiO2/PSS 90–120 4600b
Lee et al. 
200 1 CuO/ZnO/Al2O3 Carbon molecular sieve o20 – Sà et al. 
350 6 Cu/ZnO/Al2O3 Composite Pd/PSS n.d. 60000a
Lin and Rei 
– – – – o1 30000b
Han et al. 
350 6 Cu-based Composite Pd/PSS n.d. 47000b
Lin et al. 
250 5 CuO/ZnO/Al2O3 dense self-supported Pd–Ag o10 1000b
Israni and Harold 
300 3,5 CuO/Al2O3/ZnO/MgO dense self-supported Pd–Ag o10 – Iulianelli et al. 
T [1C] p [bar] Catalyst CO level in the
reformed stream [ppm]
200 1 CuO–MnO 71 Ouzounidou et al. 
180 1 CuO/ZnO/Al2O3 500b
Pan et al. 
420 1 ZnO/Al2O3 E7400b
Yang et al. 
300 1 Cu/ZnO/Al2O3 E8000b
Patel et al. 
250 1 Cu/ZnO/Al2O3 E1000b
Purnama et al. 
250 1 Cu/ZrO2 E100b
Ritskopf et al. 
100 150 200 250 300 350 400 450 500 550 600
Chiu et al.  - CR
Du et al.  - CR
Chang et al.  - CR
Durka et al.  - CR
Zhang et al.  - CR
Sanches et al.  - CR
Jones et al.  - CR
Yanga et al.  - CR
Qi et al.  - CR
Ghasemzadeh et al.  - MR
Ghasemzadeh et al.  - MR
Basile et al.  - MR
Israni and Harold  - MR
Sà et al.  - MR
Ouzounidou et al.  - MR
Zhang et al.  - MR
Lee et a.  - MR
Fig. 6. Methanol conversion vs reaction temperature for MSR reaction: comparison among literature data for both CRs and MRs [124-130,132,133].
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368
lower than 20 ppm. Therefore, as shortly resumed in Table 3, the CO
level of the reformed streams coming from CRs are not adequate to
directly supply LT-PEMFCs, needing further separation/puriﬁcation of
the hydrogen rich-streams. On the contrary, the reformed stream can
be useful for HT-PEMFCs, being the CO level lower than 20,000 ppm
and, then, in accordance with the HT-PEMFCs CO tolerance require-
ments . Concerning MRs, as shown in Table 3, the CO level in the
permeate streams depends on the kind of membrane housed inside
the MR. So, dense self-supported Pd-based membranes allow high
purity of permeated hydrogen and, as a consequence, low CO level
(o10 ppm), making possible the hydrogen supply to LT-PEMFCs.
Unfortunately, the great values of low CO concentration of
the permeated hydrogen of dense Pd-based membranes are in
contrast with the cost its-self of the membranes. Therefore, many
researchers are involved to ﬁnd a compromise between high
purity permeated hydrogen and dense Pd-based membrane cost.
However, in some case the retentate stream of such MRs shows CO
concentrations lower than 20,000–30,000 ppm, usually recog-
nized as a set tolerance for HT-PEMFCs . In that case, both
the permeate and retentate streams could be useful for LT-PEMFCs
and HT-PEMFCs supply, respectively.
6. MSR-FC integration
As above introduced, fuel cells are very efﬁcient for converting
chemical into electric energy and hydrogen is the ideal fuel for this
application. However, hydrogen has low energy density making
it difﬁcult to store and transport. Furthermore, an entirely new
distribution infrastructure and storage is needed . Previous
reasons directed the scientiﬁc community to search for new
energy vectors and methanol demonstrated to be good alternative
. In fact, it has higher energy density than hydrogen, it is
easier to handle and store and, especially, it shows relatively low
reforming temperature (240–260 1C) due to absence of C–C bonds.
As a result, many authors have been studying the MSR for in situ
hydrogen production to feed fuel cells. Commercial power supplies
are already available combining in situ hydrogen generation by
MSR to supply high temperature fuel cells, namely by Ultracell
, AixCellSys  and Serenergy . The fuel cell and the
reformer upon the closeness can be deﬁned as external reforming
(the MSR operated as standalone system) or internal reforming
(the MSR is part of the fuel cell stack) .
6.1. External reforming
Methanol steam reforming for in situ hydrogen production for
fuel cell applications has been studied mostly as a stand-alone
process. An external reformer system consists of a combustor
where a small fraction of fuel is burned and provides heat for the
following steps, a vaporizer to heat and vaporize the fuel, a
reformer to carry out the reforming reaction and a carbon
monoxide converter to carbon dioxide such as a preferential
oxidation (PROX) reactor (Fig. 7). Hydrogen puriﬁcation can be
achieved by pressure swing adsorption (PSA) or metal membrane
AixCellSys [140,143] and Serenergy  used similar strate-
gies to produce power supplies that combine external reforming
and HT-PEMFC. These systems integrate a combustor, which burns
the non-reacted hydrogen from the fuel cell out-stream, a vapor-
izer to heat and vaporize the fuel (water/methanol molar ratio of
1.5:1), a reformer loaded with CuO/ZnO/Al2O3 and HT-PEMFC
(Fig. 8). These power supplies do not require CO removal due to
the high CO tolerance of HT-PEMFC, up to ca. 1% for fuel cells
operating at 170 1C or above . The start-up period is slightly
longer for HT-PEMFC systems (5–15 min) due to the acid nature
of polymeric membranes (polybenzimidazole—PBI) that requires
materials suitable for operating under corrosive conditions, increas-
ing the size of the fuel cell stack [145,146]. During the start-up
period, a lithium battery provides the energy for two heaters until
the operation temperature is reached. Both systems are compact
and represent an important step towards the commercialization of
power supplies based on MSR/FC systems. However, the maximum
electric power output is 0.2 W cm2
for both systems , which
is half of the performance for a fuel cell fed with pure hydrogen.
Power supplies combining low temperature PEMFC and MSR
are also described in literature and commercially available. H2
planet offers a power supply with this technology  and Honda
proposed a prototype of a car equipped with a MSR-LT-PEMFC
. The International Organization for Standardization (ISO
14687) recommends for road vehicles application a maximum
CO concentration of 0.2 ppm for feeding LT-PEMFC , which
requires the reformate deep puriﬁcation. This is conventionally
achieved coupling to the MSR-CRs a WGS and a PROX reactors
, even though palladium membranes being considered with
CO2 does not affect poison the fuel cell catalyst like CO, since
dilutes further the hydrogen originating losses of ca. 20% in the
maximum power density . CO2 concentration increases as the
reformate stream progresses inside the fuel cell up to a point
where fuel starvation occurs. This fuel starvation normally hap-
pens well before the maximum power density when pure hydro-
gen is supplied. To partially compensate this drawback, a high feed
PEM Fuel Cell
Fig. 7. Standard setup for external reforming (adapted from ).
Fig. 8. Integrated MSR-FC, (adapted from ).
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368 363
ﬂow rate is supplied that originates a signiﬁcant hydrogen waste of
ca. 30% .
The external integration simpliﬁes the addition of new compo-
nents to the system that can improve the process overall efﬁciency.
As previously mentioned, an ideal reformer should produce a
hydrogen stream, mostly free of CO, and containing low concentra-
tions of CO2, methanol and water. This can be achieved using a Pd-
based reformer that allows the selective removal of hydrogen from
the reaction medium . As previously reported in the text, besides
originating a hydrogen pure stream, a Pd-based MR allows improving
the methanol conversion since hydrogen product is selectively
removed and the backward reaction is prevented . Though very
attractive, hydrogen permeates the membrane if a very low hydrogen
partial pressure is maintained in the permeate side, which can be
costly. Instead of selectively removing hydrogen, CO2 removal could
be considered and, since CO2 concentration in air is quite low, ca.
400 ppm, its use as sweep gas would provide an effective low cost
permeation driving force. For fuel cells with low sensitivity towards
CO such as HT-PEMFC, carbon dioxide removal would be the best.
However, there is still no CO2 selective membrane that can operate at
reforming temperatures through recent efforts [148,151,152]. Alter-
natively, the use of adsorbents such as zeolite 13X  and hydro-
calcites  are referred in the literature as being able to remove
selectively carbon dioxide from the reaction medium or from the
reformate stream. However, after saturation the regeneration step is
difﬁcult to accomplish. A thermal swing adsorption (TSA) process
could in principle be considered for purifying the reformate stream
but this is normally an energy demanding process .
The thermal resistance between the heat source and catalyst bed
must be as small as possible. For external reforming integration the
heat required for the reforming process is typically provided by a
combustor [4,157]. The ﬂow and heat transfer (combustor–reformer)
effect on the reactor performance has been studied using phenom-
enological models [156,158,159]. Heat conduction through the micro-
reactors walls was observed to have a signiﬁcant impact on the
temperature distribution and consequently on the methanol conver-
sion . Thus, to optimize the heat transfer high conductive
materials should be used on combustor and reformer fabrication.
The heat transfer is also affected by different designs adopted for
combustors and reformers. For example, by changing reformer and
combustor from parallel channel design to serpentine, the ﬂow
velocity increases and, then, the stagnant ﬁlm adjacent to the wall
becomes thinner and the heat transfer coefﬁcient increases [156,158].
A more efﬁcient heat transfer from the combustor to the reformer
allows higher hydrogen yields. In small devices the heat manage-
ment is critical because the high surface-to-volume ratio. A cylind-
rical design organized in a “thermal cascade” can be adopted to
minimize the heat losses, having cooler layers covering hotter ones,
thus the combustor is inserted in the center followed by the
vaporizer, the reformer and so on [161,162].
External reforming has the advantage of being not restricted to
a reformer/fuel cell stack conﬁguration, allowing different designs
potentially more efﬁcient for fuel processing. The reformer can
operate at higher temperatures and a MR conﬁguration can be
used, which results in higher conversions and the production of a
puriﬁed hydrogen stream.
6.2. Internal reforming
Internal reforming involves heat and mass exchange between
the MSR and electrochemical reaction and it is classiﬁed as direct
or indirect, depending on the MSR catalyst if inserted or not in the
anode compartment, respectively .
Fuel cells are exothermic devices that waste ca. 50% of the input
chemical energy as heat, while methanol steam reformers are
endothermic; internal reforming targets to take advantage of efﬁcient
heat exchange between the two devices. LT-PEMFCs operate at ca.
80 1C and HT-PEMFCs at ca. 180 1C, while MSR operates at ca. 250 1C.
Due to this mismatching operating temperature, many authors
choose external reforming, but for HT-PEMFC a synergetic heat
integration can be achieved if possible either or both to increase
the fuel cell operating temperature or lower the reforming tempera-
ture. Since the operation of HT-PEMFC is limited to a maximum
operating temperature of 200 1C, a few authors proposed lowering
the reforming temperature [37,103,163]. At 180 1C the methanol
conversion in a commercial catalyst (CuO/ZnO/Al2O3) is very low.
For example, for a contact time of Wcat/FMeOH¼30 kg s mol1
methanol conversion is 80% at 250 1C and 13% at 180 1C .
Pan et al.  were as ﬁrst authors to study the performance of
an indirect internal reforming coupled with a HT-PEMFC operating
at 180–200 1C. They loaded the reformer with 149 g of commercial
catalyst (CuO/ZnO/Al2O3) and obtained a hydrogen yield of 400 dm3
for nearly 100% of methanol conversion. The fuel cell
stack exhibited a lower maximum power density when fed with
reformate compared to when fed with pure hydrogen but a higher
energy efﬁciency .
Avgouropoulos et al. [165,166] used a fuel cell equipped with a PBI
electrolyte membrane by ADVENT TPS that resists to higher tem-
peratures, up to 210 1C, and a methanol reforming catalyst of
CuMnOx loaded in the anode chamber (Fig. 9). The system was
operated at 200–210 1C producing a current density of 0.17 A cm2
at 600 mV. The advantages of the indirect internal reforming are
compactness and heat integration. The reforming conversion is also
enhanced by the continuous electrochemical hydrogen removal from
the reforming reaction medium. However, since PBI membranes are
intolerant to high methanol concentrations, resulting in low power
The production of MSR reaction still continues to be an active
area of research and much progress has been achieved both in the
ﬁeld of catalysts development and applications involving both CRs
Fig. 9. Direct Internal MSR (adapted from ).
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368
and MRs, even though many problems still remain to be solved.
This review deals with MSR reaction to produce hydrogen for
PEMFC supply combined to an overview on the new ﬁndings on
MSR catalyst development and inorganic MR technology. In parti-
cular, it is reasonable to understand that the exploitation of renew-
able sources such as methanol constitutes an important possibility
in the route of hydrogen production via reforming reactions by
inorganic MR technology. This combination could drive to an
improvement of the hydrogen production units, making possible
the requirements for the integration of methanol-based fuel pro-
cessors with PEM fuel cells. A critic issue not largely addressed in
the specialized literature involves this concept: considering that
natural gas and, more in general, other derived fossil fuels are
essentially utilized for stationary applications, it is expected that
alcohols such as methanol could have a major impact on the future
portable applications. However, reactor and system development
activities by several scientiﬁc groups around the world demon-
strated the ability of performing MSR reaction at small and large
scale and at high efﬁciencies. As a consequence, selection of
material and system design vary a lot from the very small metal,
glass or ceramic micro-reactors to the large scale, high pressure
membrane-based systems. In the area of inorganic MRs applied to
MSR reaction, a relevant still unsolved issue is represented by the
impossibility of comparing the performances (in terms of conver-
sion, hydrogen yield and hydrogen recovery) among the existing
scientiﬁc works owing to the different operating conditions adopted
by each author during the experimental tests. Furthermore, even
though in literature there are a number of studies on MSR reaction
performed in MRs, no one of them focuses on cost analysis of
these devices. This aspect points out that inorganic MR technology
still presents some deﬁciencies to be overcome before its imple-
mentation at larger scales. As a future perspective, a new research
approach should be aimed by the preparation of composite mem-
branes based on very thin Pd-layer deposited onto porous supports
showing very high hydrogen/other gas perm-selectivity, able to
operate for long periods at high temperatures and pressures as well
as to develop membrane systems not based on palladium by
exploiting the potentiality of HT-PEMFCs to tolerate higher level of
CO in the hydrogen stream supplied.
Major advances have been made in the ﬁeld of hydrogen
production through MSR. New catalyst base on cooper or/and
palladium are being developed and is expected higher catalytic
activity, making possible the complete integration of MSR-reactors
with PEMFC. Tubular reactors or coil designs cause high pressure
drops and are not the most suitable for MSR reaction, others
designs as radial demonstrate being more appropriate. MRs play
an important role in hydrogen production, promising weight and
space savings. Dense metal membranes provide high purity
hydrogen over a wide range of pressure and temperature. The
selective removal of hydrogen enhances the methanol conversion
that is higher than the conversion in a conventional reactor. But
the futures of membrane reactors for fuel cell depends on the
ability to produce high permeate ﬂuxes at low system pressure
with moderate cost and suitable stability in all phases of a typical
The research leading to these results has received funding from
the European Union′s Seventh Framework Programme (FP/2007-
2013) for the Fuel Cells and Hydrogen Joint Technology Initiative
under grant agreement no.  10.
 Wee J. Applications of proton exchange membrane fuel cell systems. Renew-
able Sustainable Energy Reviews 2007;11:1720–38.
 Bose S, Kuila T, Nguyen TXH. Polymer membranes for high temperature
proton exchange membrane fuel cell: recent advances and challenges.
Progress in Polymer Science 2011;36:813–43.
 Heinzel A, Vogel B, Hiugner P. Reforming of natural gas hydrogen genera-
tion for small scale stationary fuel cell systems. Journal of Power Sources
 Chein RY, Chen YC, Lin YS, Chung JN. Hydrogen production using integrated
methanol-steam reforming reactor with various reformer designs for PEM
fuel cells. International Journal of Hydrogen Energy 2012;36:466–76.
 Pettersson LJ, Westerholn R. State of the art of multi-fuel reformers for fuel
cell vehicles: problem identiﬁcation and research needs. International
Journal of Hydrogen Energy 2001;26:243–64.
 Lindström B, Pettersson LJ. Development of a methanol fuelled reformer for
fuel cell applications. Journal of Power Sources 2003;118:71–8.
 Han J, Kim IS, Choi KS. Puriﬁer-integrated methanol reformer for fuel cell
vehicles. Journal of Power Sources 2000;86:223–7.
 Lu GQ, Diniz de Costa JC, Duke M, Giessler S, Socolow R, Williams RH, et al.
Inorganic membranes for hydrogen production and puriﬁcation: a critical review
and perspective. Journal of Colloid and Interface Science 2007;314:589–603.
 Xiu S, Shahbazi A. Bio-oil production and upgrading research: a review.
International Journal of Hydrogen Energy 2012;16:4406–14.
 Basile, A, Iulianelli, A, Longo, T, Liguori, S, De Falco, M. Pd-based selective
membrane State-of-the-Art. In: Membrane reactors for hydrogen production
processes, L Marrelli, M De Falco G Iaquaniello, editors, Springer London
Dordrecht Heidelberg New York; 2011 Chapter 2, pp. 21–55, ISBN 978-0-
 Wieland S, Melin T, Lamm A. Membrane reactors for hydrogen production.
Chemical Engineering Science 2002;57:1571–6.
 Damle AS. Hydrogen production by reforming of liquid hydrocarbons in a
membrane reactor for portable power generation—experimental studies.
Journal of Power Sources 2009;186:167–77.
 Iulianelli, A, Liguori, S, Longo, T, Basile, A. Inorganic membrane and
membrane reactor technologies for hydrogen production. in: Hydrogen
production: prospects and processes, Damon Robert Honery and Patrick
Moriarty, editors, Victoria, Australia, Nova Science Publishers, Series: Energy
Science, Engineering and Technology, isbn:978-1-62100-246-8; 2012. Chap-
ter 12, pp. 377–398.
 Basile A. Hydrogen production using Pd-based membrane reactors for fuel
cells. Topics in Catalysis 2008;51:107–22.
 Lin YM, Rei MH. Process development for generating high purity hydrogen
by using supported palladium membrane reactor as steam reformer. Inter-
national Journal of Hydrogen Energy 2000;25:211–9.
 Mallada R, Menéndez M. Inorganic membranes: synthesis, characterization
and applications. Technology Engineering 2008:460.
 Saracco G, Specchia V. Catalytic inorganic membrane reactors: present
experience and future opportunities. Catalysis Reviews-science and Engi-
 Shu J, Grandjean BPA, Van Neste A, Kaliaguine S. Catalytic palladium-based
membrane reactors: a review. The Canadian Journal of Chemical Engineering
 Grashoff GJ, Pilkington CE, Corti CW. The puriﬁcation of hydrogen—a review
of the technology emphasizing, the current status of palladium membrane
diffusion. Platinum Metals Review 1983;27:157–68.
 Hsieh HP. Inorganic membrane reactors—a review. AIChE Symposium Series
 Tong J, Shirai R, Kashima Y, Matsumura Y. Preparation of a pinhole-free Pd–
Ag membrane on a porous metal support for pure hydrogen separation.
Journal of Membrane Science 2005;260:84–9.
 Adhikari S, Fernand S. Hydrogen membrane separation techniques. Indus-
trial Engineering Chemistry Research 2006;45:875–81.
 Arstad B, Venvik H, Klette H, Walmsley JC, Tucho WM, Holmestad R, et al. Studies
of self-supported 1.6 μm Pd/23 wt% Ag membranes during and after hydrogen
production in a catalytic membrane reactor. Catalysis Today 2006;118:63–72.
 Dolan MD, Dave NC, Ilyushechkin AY, Morpeth LD, McLennan KG. Composi-
tion and operation of hydrogen-selective amorphous alloy membranes.
Journal of Membrane Science. 2006;285:30–55.
 Falconer JL, Noble RD, Sperry DP. Catalytic membrane reactors. In: Noble RD,
Stern SA, editors. Membrane separations technology: principles and applica-
tions. Elsevier; 1995. p. 669–712.
 Sà S, Sousa JM, Mendes A. Methanol steam reforming in a dual-bed
membrane reactor for producing PEMFC grade hydrogen. Catalysis Today
 Agrell J, Birgersson H, Boutonnet M. Steam reforming of methanol over a
Cu/ZnO/Al2O3 catalyst: a kinetic analysis and strategies for suppression of CO
formation. Journal of Power Sources 2002;106(1–2):249–57.
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368 365
 Jiang CJ, Trimm DL, Wainwright MS, Cant NW. Kinetic study of steam
reforming of methanol over copper-based catalysts. Applied Catalysis A:
 Jiang CJ, Trimm DL, Wainwright MS, Cant NW. Kinetic mechanism for the
reaction between methanol and water over a Cu–ZnO–Al2O3 catalyts.
Applied Catalysis A: General 1993;97(2):145–58.
 Schuessler M, Lamla O, Stefanovsky T, Klein C, zur Megede D. Autothermal
reforming ofmethanol in an isothermal reactor—concept and realisation.
Chemical Engineering Technology 2001;24(11):1141–5.
 Takahashi T, Inoue M, Kai T. Effect of metal composition on hydrogen
selectivity in steam reforming of methanol over catalysts prepared from
amorphous alloys. Applied Catalysis A: General 2001;218:189–95.
 Sekizawa K, Yano S, Eguchi K, Arai H. Selective removal of CO in methanol
reformed gas over Cu-supported mixed metal oxides. Applied Catalysis A:
 Alejo L, Lago R, Peňa MA, Fierro JLG. Partial oxidation of methanol to produce
hydrogen over Cu–Zn-based catalysts. Applied Catalysis A: General 1997;162:
 Shen GC, Fujita S, Matsumoto S, Takezawa N. Steam reforming of methanol
on binary Cu/ZnO catalysts: effect of preparation condition upon precursor,
surface structure and catalytic activity. Journal of Molecular Catalysis A:
 Reitz TL, Ahmed S, Krumpelt M, Kumar R, Kung HH. Characterization of
CuO/ZnO under oxidizing conditions for the oxidative methanol reforming
reaction. Journal of Molecular Catalysis A: Chemical 2000;162:275–85.
 Velu S, Suzuki K, Kapoor MP, Ohashi F, Osaki T. Selective production of
hydrogen for fuel cells via oxidative steam reforming of methanol over
CuZnAl (Zr)-oxide catalysts. Applied Catalysis A: General 2001;213:47–63.
 Chein R-Y, Chen Y-C, Lin Y-S, Chung JN. Experimental study on the hydrogen
production of integrated methanol-steam reforming reactors for PEM fuel
cells. International Journal of Thermal Sciences 2011;50:1253–62.
 Palo D, Dagle R, Holladay J. Methanol steam reforming for hydrogen
production. Chemical Reviews 2007;107:3992–4021.
 Turco M, Bagnasco G, Cammarano C, Senese P, Costantino U, Sisani M. Cu/
ZnO/Al2O3 catalysts for oxidative steam reforming of methanol: the role of
Cu and the dispersing oxide matrix. Applied Catalysis B: Environmental
 Mastalir Á, Patzkó Á, Frank B, Schomäcker R, Ressler T, Schlögl R. Steam
reforming of methanol over Cu/ZnO/Al2O3 modiﬁed with hydrotalcites.
Catalysis Communications 2007;8:1684–90.
 Conant T, Karim A, Lebarbier V, Wang Y, Girgsdies F, Schlögl R, et al. Stability
of bimetallic Pd–Zn catalysts for the steam reforming of methanol. Journal of
 Jeong H, Kimb KI, Kimb TH, Ko CH, Park HC, Song IK. Hydrogen production by
steam reforming of methanol in a micro- channel reactor coated with Cu/
ZnO/ZrO2/Al2O catalyst. Journal of Power Sources 2006;159:1296–9.
 Yong-Feng L, Xin-Fa D, Wei-Ming L. Effects of ZrO2-promoter on catalytic
performance of CuZnAlO catalysts for production of hydrogen by steam
reforming of methanol,. International Journal of Hydrogen Energy
 Ma L, Gong B, Tran T, Wainwright MS. Cr2O3 promoted skeletal Cu catalysts
for the reactions of methanol steam reforming and water gas shift. Catalysis
 Clancy P, Breen J, Ross J. The preparation and properties of coprecipitated
Cu–Zr–Y and Cu–Zr–La catalysts used for the steam reforming of methanol.
Catalysis Today 2007;127:291–4.
 Shishido T, Yamamoto Y, Morioka H, Takaki K, Takehira K. Active Cu/ZnO and Cu/
ZnO/Al2O3 catalysts prepared by homogeneous precipitation method in steam
reforming of methanol. Applied Catalysis A: General 2004;263:249–53.
 Jakdetchai O, Takayama N, Nakajima T. Activity enhancement of CuZn-
impregnated Fsm-16 by modiﬁcation with 1,3-butanediol for steam reform-
ing of methanol. Kinetics and Catalysis 2005;46:56–64.
 Lindström B, Pettersson LJ, Menon PG. Activity and characterization of Cu/Zn,
Cu/Cr and Cu/Zr on γ-alumina for methanol reforming for fuel cell vehicles.
Applied Catalysis A: General 2002;234:111–25.
 Papavasiliou J, Avgouropoulos G, Ioannides T. Reforming of methanol over
copper–manganese spinel oxide catalysts. Catalysis Communications 2005;6:
 Oguchi H, Nishiguchi T, Matsumoto T, Kanai H, Utani K, Matsumura Y, et al.
Steam reforming of methanol over Cu/CeO2/ZrO2 catalysts. Applied Catalysis
A: General 2005;281:69–73.
 Liu Y, Hayakawa T, Tsunoda T, Suzuki K, Hamakawa S, Murata K, et al. Steam
reforming of methanol over Cu/CeO2 catalysts studied in comparison with
Cu/ZnO and Cu/Zn(Al)O catalysts. Topics in Catalysis 2003;22:205–13.
 Agrell J, Birgersson H, Boutonnet M, Melián-Cabrera I, Navarro R, Fierro J.
Production of hydrogen from methanol over Cu/ZnO catalysts promoted by
ZrO2 and Al2O3. Journal of Catalysis 2003;219:389–403.
 Liu Q, Wang L-C, Chen M, Liu Y-M, Cao Y, He H-Y, et al. Waste-free soft
reactive grinding synthesis of high-surface-area copper–manganese spinel
oxide catalysts highly effective for methanol steam reforming. Catalysis
 Yao C-Z, Wang L-C, Liu Y-M, Wu G-S, Cao Y, Dai W-L, et al. Effect of
preparation method on the hydrogen production from methanol steam
reforming over binary Cu/ZrO2 catalysts. Applied Catalysis A: General
 Marbán G, Valdés-Solís T, Fuertes AB. High surface area CuMn2O4 prepared
by silica-aquagel conﬁned co-precipitation. Characterization and testing in
steam reforming of methanol. Catalysis Letters 2007;118:8–14.
 Yang H-M, Liao P-H. Preparation and activity of Cu/ZnO–CNTs nano-catalyst on
steam reforming of methanol. Applied Catalysis A: General 2007;317:226–33.
 Gao L, Sun G, Kawi S. A study on methanol steam reforming to CO2 and H2 over
the La2CuO4 nanoﬁber catalyst. Journal of Solid State Chemistry 2008;181:7–13.
 Iwasa N, Masuda S, Takezawa N. Steam reforming of methanol over Pd/ZnO:
effect of the formation of PdZn alloys upon the reaction. Reaction Kinetics
and Catalysis Letters 1995;55:349–53.
 Iwasa N, Mayanagi T, Masuda S, Takezawa N. Steam reforming of methanol
over PdZn catalysts. Reaction Kinetics and Catalysis Letters 2000;69:355–60.
 Iwasa N, Kudo S, Takahashi H, Masuda S, Takezawa N. Highly selective
supported Pd catalyst for steam reforming of methanol. Catalysis Letters
 Iwasa N, Mayanagi T, Nomura W, Arai M, Takezawa N. Effect of Zn addition to
supported Pd catalyst in the steam reforming of methanol. Applied Catalysis
A: General 2003;248:153–60.
 Chin YH, Wang Y, Dagle RA, Li XS. Methanol steam reforming over Pd/ZnO:
catalyst preparation and pretreatment studies. Fuel Processing Technology
 Qi C, Amphlett JC, Peppley BA. Methanol steam reforming over NiAl and NiAl
(Au, Rh, Ir)-layered double hydroxide derived catalysts. Catalysis Letters
 Karim A, Conant T, Datye A. The role of PdZn alloy formation and particle
size on the selectivity for steam reforming of methanol. Journal of Catalysis
 Sá S, Silva H, Brandão L, Sousa J, Mendes A. Catalysts for methanol steam
reforming—a review. Applied Catalysis B: Environmental 2010;99:43–57.
 Hessel V, Hardt S, Lowe H. Chemical micro processing engineering, funda-
mentals, modelling and reactions. Weinheim: Wiley-VCH, Verlag GmbH;
 Checchetto R, Bazzanella N, Patton B, Miotello A. Palladium membranes
prepared by r.f. magnetron sputtering for hydrogen puriﬁcation. Surface and
Coatings Technology 2004;177–178:73–9.
 An H, Angli A, Agus B, Sasmito P, Jundika C, Kurnia A, et al. Computational
ﬂuid dynamics (CFD) analysis of micro-reactor performance: effect of various
conﬁgurations. Chemical Engineering Science 2012;75:85–95.
 Jang J, Cheng C, Huang Y, Lee C, Leu C. Optimal design of parallel channel
patterns in a micro methanol steam reformer. International Journal of
Hydrogen Energy 2012;37:16974–85.
 Pattekar A, Kothare M. A microreactor for hydrogen production in micro fuel
cell applications. Journal of Microelectromechanical Systems 2004;13:7–18.
 Telotte J, Kern J, Palanki S. Miniaturized methanol reformer for fuel cell
powered mobile applications. International Journal of Chemical Reactor
 Karim A, Bravo J, Datye A. Non isothermally in packed bed reactors for steam
reforming of methanol. Applied Catalysis A: General 2005;282:101–9.
 Perng S, Horng R, Ku H. Effects of reaction chamber geometry on the
performance and heat/mass transport phenomenon for a cylindrical metha-
nol steam reformer. Applied Energy 2012.
 Suh J, Lee M, Greif R, Costas P. Grigoropoulos, transport phenomena in a
steam-methanol reforming microreactor with internal heating. International
Journal of Hydrogen Energy 2009;34:314–22.
 Terazaki T, Nomura M, Takeyama K, Nakamura O, Yamamoto T. Development
of multi-layered micro-reactor with methanol reformer for small PEMFC.
Journal of Power Sources 2005;145:691–6.
 Kawamura Y, Ogura N, Yamamoto T, Igarashi A. A miniaturized methanol
reformer with Si-based microreactor for a small PEMFC. Chemical Engineer-
ing Science 2006;61:1092–101.
 Oh S, Kim J. Method of catalyst coating in micro-reactors for methanol steam
reforming. Applied Catalysis A: General 2007;316:83–9.
 Karim A, Bravo J, Gorm D, Conant T, Datye A. Comparison of wall-coated and
packed-bed reactors for steam reforming of methanol. Catalysis Today
 Bravo J, Karim A, Conant T, Lopez G, Datye A. Wall coating of a CuO/ZnO/
Al2O3 methanol steam reforming catalyst for micro-channel reformers.
Chemical Engineering Journal 2004;101:113–21.
 Lee M, Greif R, Costas P, Grigoropoulos H, Park F Hsu. Transport in packed-
bed and wall-coated steam-methanol reformers. Journal of Power Sources
 Pan M, Wei X, Tang Y. Factors inﬂuencing methanol steam reforming inside
the oriented linear copper ﬁber sintered felt. International Journal of
Hydrogen Energy 2012;37:11157–66.
 Soria R. Overview on industrial membranes. Catalysis Today 1995;25(3–
 Westermann T, Melin T. Review – ﬂow-through catalytic membrane reactors
– Principles and applications. Chemical Engineering and Processing
 Lin YS. Microporous and dense inorganic membranes: current status and
prospective. Separation and Puriﬁcation Technology 2001;25:39–55.
 McLeary EE, Jansen JC, Kapteijn F. Zeolite based ﬁlms, membranes and
membrane reactors: progress and prospects. Mesopotamia Mathematics
 Fong YY, Abdullah AZ, Ahmad AL, Bhatia S. Review—development of
functionalized zeolite membrane and its potential role as reactor combined
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368
separator for para-xylene production from xylene isomers. Chemical Engi-
neering Journal 2008;139:172–93.
 Huang J, El-Azzami LA, Ho WSW. Modeling of CO2-selective water gas shift
membrane reactor for fuel cell. Journal of Membrane Science 2005;261:67–75.
 Scholes CA, Smith KH, Kentish SE, Stevens GW. Review – CO2 capture from
pre-combustion processes – strategies for membrane gas separation. Inter-
national Journal of Greenhouse Gas Control 2010;4:739–55.
 Andrić P, Meyer AS, Jensen PA, Johansen KD. Reactor design for minimizing
product inhibition during enzymatic lignocellulose hydrolysis II. Quantiﬁca-
tion of inhibition and suitability of membrane reactors. Biotechnology
 Reij MW, Keurentjes JTF, Hartmans S. Review—membrane bioreactors for
waste gas treatment. Journal of Biotechnology 1998;59:155–67.
 Woodside SM, Bowen BD, Piret JM. Mammalian cell retention devices for
stirred perfusion bioreactors. Cytotechnology 1998;28:163–75.
 Chatenet M, Dubau L, Job N, Maillard F. The (electro) catalyst membrane
interface in the proton exchange membrane fuel cell: similarities and
differences with non-electrochemical catalytic membrane reactors. Catalysis
 Mozia S. Photocatalytic membrane reactors (PMRs) in water and wastewater
treatment: a review. Separation and Puriﬁcation Technology 2010;73:71–91.
 Dittmeyer R, Höllein V, Daub K. Membrane reactors for hydrogenation and
dehydrogenation processes based on supported palladium. Journal of Mole-
cular Catalysis A: Chemical 2001;173(1–2):135–84.
 Saracco G, Neomagus HWJP, Versteeg GF, van Swaaij WPM. High-
temperature membrane reactors: potential and problems. Chemical Engi-
neering Science 1999;54:1997–2017.
 Coronas J, Santamaria J. Catalytic reactors based on porous ceramic mem-
branes. Catalysis Today 1999;51:377–89.
 Edlund DJ, Pledger WA. Thermolysis of hydrogen sulﬁde in a metal-
membrane reactor. Journal of Membrane Science 1993;77:255–64.
 Li A, Liang W, Hughes R. The effect of carbon monoxide and steam on the
hydrogen permeability of a Pd/stainless steel membrane. Journal of Mem-
brane Science 2000;165:135–41.
 Amandusson H, Ekedahl LG, Dannetun H. The effect of CO and O2 on
hydrogen permeation through a palladium membrane. Applied Surface
 McCool BA, Lin YS. Nanostructured thin palladium-silver membranes: effects
of grain size on gas permeation properties. Journal of Materials Science
 Uemiya S. State-of-art-the-art of supported metal membranes for gas
separation. Separation and Puriﬁcation Technology 1999;28:51–85.
 Peighambardoust SJ, Rowshanzamir S, Amjadi M. Review of the proton
exchange membranes for fuel cell applications. International Journal of
Hydrogen Energy 2010;35:9349–84.
 Pan C, He R, Li Q, Jensen J, Bjerrum N, Hjulmand H. Integration of high
temperature PEM fuel cells with a methanol reformer. Journal of Power
 Iulianelli A, Basile A. Sulfonated PEEK-based polymers in PEMFC and DMFC
applications: a review. International Journal of Hydrogen Energy 2012;37
 Israni S, Harold MP. Methanol steam reforming in single-ﬁber bed Pd–Ag
membrane reactor: experiments and modeling. Journal of Membrane Science
 Rei MH, Yeh GT, Tsai YH, Kao YL, Shiau LD. Catalysis-spillover-membrane. III:
The effect of hydrogen spillover on the palladium membrane reactor in the
steam reforming reactions. Journal of Membrane Science 2011;369:299–307.
 Sà S, Sousa JM, Mendes A. Steam reforming of methanol over a CuO/ZnO/
Al2O3 catalyst Part II: A carbon membrane reactor. Chemical Engineering
 Lee DW, Nam SE, Sea B, Ihm SK, Lee KH. Preparation of Pt-loaded hydrogen
selective membranes for methanol reforming. Catalysis Today 2006;118:
 Lin YM, Rei MH. Study on hydrogen production from methanol steam reforming
in supported palladium membrane reactor. Catalysis Today 2001;67:77–84.
 Basile A, Tosti S, Capannelli G, Vitulli G, Iulianelli A, Gallucci F, et al. Co-
current and counter-current modes for methanol steam reforming mem-
brane reactor: experimental study. Catalysis Today 2006;118:237–45.
 Lee DW, Park SJ, Yu CY, Ihm SK, Lee KH. Study on methanol reforming-
inorganic membrane reactors combined with water-gas shift reaction and
relationship between membrane performance and methanol conversion.
Journal of Membrane Science 2008;316:63–72.
 Briceño K, Iulianelli A, Montanè D, Garcia-Valls R, Basile A. Carbon molecular
sieve membranes supported on non-modiﬁed ceramic tubes for hydrogen
separation in membrane reactors. International Journal of Hydrogen Energy
 Zhang X, Hu H, Zhu Y, Zhu S. Methanol steam reforming to hydrogen in a
carbon membrane reactor system. Industrial Engineering Chemistry
 Iulianelli A, Longo T, Basile A. Methanol steam reforming in a dense Pd–Ag
membrane reactor: the pressure and WHSV effects on CO-free H2 production.
Journal of Membrane Science 2008;323:235–40.
 Itoh N, Kaneko Y, Igarashi A. Efﬁcient hydrogen production via methanol
steam reforming by preventing back-permeation of hydrogen in a palladium
membrane reactor. Industrial Engineering Chemistry Research
 Briceño K, Montanè D, Garcia-Valls R, Iulianelli A, Basile A. Fabrication
variables affecting the structure and properties of supported carbon mole-
cular sieve membranes for hydrogen separation. Journal of Membrane
 Lin YM, Lee GL, Rei MH. An integrated puriﬁcation and production of
hydrogen with a palladium membrane-catalytic reactor. Catalysis Today
 Han J, Kim IS, Choi KS. High purity hydrogen generator for on-site hydrogen
production. International Journal of Hydrogen Energy 2002;27:1043–7.
 Han J, Lee SM, Chang H. Metal membrane-type 25-kW methanol fuel processor
for fuel cell hybrid vehicle. Journal of Power Sources 2002;112:484–90.
 Iulianelli A, Longo T, Basile A. Methanol steam reforming reaction in a Pd–Ag
membrane reactor for CO-free hydrogen production. International Journal of
Hydrogen Energy 2008;33:5583–8.
 Ghasemzadeh K, Liguori S, Morrone P, Iulianelli A, Piemonte, V. Babaluo, A.A.
Basile A. H2production by low pressure methanol steam reforming in a dense
Pd-Ag membrane reactor in co-current ﬂow conﬁguration: experimental and
modeling analysis,accepted, International Journal of Hydrogen Energy, http://
dx.doi.org/10.1016/j.ijhydene.2013.06.001, in press.
 Ghasemzadeh, K, Liguori, S, Iulianelli, A, Morrone, P, Babaluo, AA, Basile, A. H2
production in silica membrane reactor via methanol steam reforming:
modeling and HAZOP analysis, submitted to International Journal of Hydro-
gen Energy, http://dx.doi.org/10.1016/j.ijhydene.2013.06.008.
 Basile A, Tereschenko GF, Orekhova NV, Ermilova MM, Gallucci F, Iulianelli A.
An experimental investigation on methanol steam reforming with oxygen
addition in a ﬂat Pd/Ag membrane reactor,. International Journal of Hydrogen
 Chiu K-l, Kwong F-l, Ng DHL. Oxidation states of Cu in the CuO/CeO2/Al2O3
catalyst in the methanol steam reforming process. Current Applied Physics
 Du X, Shen Y, Yang L, Shi Y, Yang Y. Experiments on hydrogen production
from methanol steam reforming in the micro-channel reactor. International
Journal of Hydrogen Energy 2012;37:12271–80.
 Chang C-C, Wanga J-W, Chang C-T, Liaw B-J, Chen Y-Z. Effect of ZrO2 on steam
reforming of methanol over CuO/ZnO/ZrO2/Al2O3 catalysts. Chemical
Engineering Journal 2012;192:350–6.
 Durka T, Stefanidis GD, Van Gerven T, Stankiewicz AI. Microwave-activated
methanol steam reforming for hydrogen production. International Journal of
Hydrogen Energy 2011;36:12843–52.
 Zhang Q, Farrauto RJ. A PdZn catalyst supported on stabilized ceria for
stoichiometric methanol steam reforming and hydrogen production. Applied
Catalysis A: General 2011;395:64–70.
 Sanches SG, Flores JH, de Avillez RR, Pais da Silva MI. Inﬂuence of preparation
methods and Zr and Y promoters on Cu/ZnO catalysts used for methanol steam
reforming. International Journal of Hydrogen Energy 2012;37:6572–9.
 Jones SD, Hagelin-Weaver HE. Steam reforming of methanol over CeO2- and
ZrO2-promoted Cu-ZnO catalysts supported on nanoparticle Al2O3. Applied
Catalysis B: Environmental 2009;90:195–204.
 Yang M, Li S, Chen G. High-temperature steam reforming of methanol over
ZnO–Al2O3 catalysts. Applied Catalysis B: Environmental 2011;101:409–16.
 Qi C, Amphlett JC, Peppley BA. Stability of NiAl layered double hydroxides
derived catalysts for the steam reforming of methanol. Catalysis Commu-
 Sà S, Silva H, Sousa JM, Mendes A. Hydrogen production by methanol steam
reforming in a membrane reactor: palladium vs carbon molecular sieve
membranes. Journal of Membrane Science 2009;339:160–70.
 Ouzounidou M, Ipsakis D, Voutetakis S, Papadopoulou S, Seferlis P.
A combined methanol autothermal steam reforming and PEM fuel cell pilot
plant unit: experimental and simulation studies. Energy 2009;34:1733–43.
 Patel S, Pant KK. Experimental study and mechanistic kinetic modeling for
selective production of hydrogen via catalytic steam reforming of methanol.
Chemical Engineering Science 2007;62:5425–35.
 Purnama H, Ressler T, Jentoft RE, Soerijanto H, Schlögl R, Schomäcker R.
CO formation/selectivity for steam reforming of methanol with a commercial
CuO/ZnO/Al2O3 catalyst. Applied Catalysis A: General 2004;259:83–94.
 Ritzkopf I, Vukojevic S, Weidenthaler C, Grunwaldt J-D, Ferdi Schüth.
Decreased CO production in methanol steam reforming over Cu/ZrO2
catalysts prepared by the microemulsion technique. Applied Catalysis A:
 Olah GA, Goeppert A, Prakash GKS. Beyond oil and gas: the methanol
economy. Weinheim (Germany): Wiley-VCH; 2006.
 [access date February 2013], 〈http://www.ultracellpower.com/sp.php?rmfc〉.
 Huck, T, Engelhardt, P, Lucka, K. Highly integrated micro fuel cell system
based on a methanol steam reformer and a HT PEM fuel cell. 15th Europeam
Fuel Cell Forum. Lucern, Switzerland; 2011.
 Andreasen S, Kær S, Sahlin S. Control and experimental characterization of a
methanol reformer for a 350 W high temperature polymer electrolyte
membrane fuel cell system international. International Journal of Hydrogen
 Qi A, Peppley B, Karan K. Integrated fuel processors for fuel cell application: a
review. Fuel Processing Technology 2007;88:3–22.
 Wichmann D, Engelhardt P, Wruck R, Lucka K, Köhne H. Development of a
highly integrated micro fuel processor based on methanol steam reforming
for a HT-PEM fuel cell with an electric power output of 30 W. ECS Transac-
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368 367
 Boaventura M, Mendes A. Activation procedures characterization of MEA
based on phosphoric acid doped PBI membranes. International Journal of
Hydrogen Energy 2010;35:11649–60.
 Juhl AS, Knudsen KS. Modelling and evaluation of heating strategies for high
temperature polymer electrolyte membrane fuel cell stacks. International
Journal of Hydrogen Energy 2008;33:4655–64.
 Kurz T, Keller J. Heat management in a portable high temperature PEM fuel
cell module with open cathode. Fuel Cells 2011;11:518–25.
 [access date February 2013] 〈http://en.wikipedia.org/wiki/Honda_FCX_Clarity〉.
 International Organization for Standardization, ISO/TS 14687-2, Hydrogen
Fuel-Product Speciﬁcation—Part 2: Proton exchange membrane Fuel Cell
applications for road vehicles; 2012.
 Yan X, Wang S, Li X, Hou M, Yuan Z, Li D, et al. A 75-kW methanol reforming
fuel cell system. Journal of Power Sources 2006;162:1265–9.
 Katiyar N, Kumar S, Kumar S. Comparative thermodynamic analysis of adsorp-
tion, membrane and adsorption-membrane hybrid reactor systems for metha-
nol steam reforming. International Journal of Hydrogen Energy 2012:1–13.
 Basile, A, Gugliuzza, A, Iulianelli, A, Morrone, P. Membrane technology for
carbon dioxide (CO2) capture in power plants. In: Advanced membrane
science and technology for sustainable energy and environmental applica-
tions, editor, A Basile and SP Nunes, Woodhead publishing Series in Energy—
Cornwall (UK), 2011, Ch. 5, pp.113-159. ISBN: 978-1-84569-969-7, ISSN:
 Iulianelli, A, Basile, A, Li, H, Van Den Brink, RW. Inorganic membranes for pre-
combustion carbon dioxide (CO2) capture. In: Advanced membrane science
and technology for sustainable energy and environmental applications,
editor, A Basile and SP Nunes, Woodhead Publishing Series in Energy—
Cornwall (UK), 2011, Ch. 7, pp 184-213. ISBN: 978-1-84569-969-7, ISSN:
 Harale A, Hwanga H, Liub P, Sahimi M, Tsotsis T. Experimental studies of a
hybrid adsorbent-membrane reactor (HAMR) system for hydrogen produc-
tion. Chemical Engineering Science 2007;62:4126–37.
 Ding Y, Alpay E. Equilibria and kinetics of CO2 adsorption on hydrotalcite
adsorbent. Chemical Engineering Science 2000;55:3461–74.
 Lee K, Beaver M, Caram H, Sircar S. Production of fuel-cell grade hydrogen by
thermal swing sorption enhanced reaction concept. International Journal of
Hydrogen Energy 2008;33:781–90.
 Hsueh C, Chu H, Yan W, Chen C. Numerical study of heat and mass transfer in
a plate methanol steam micro reformer with methanol catalytic combustor.
International Journal of Hydrogen Energy 2010;35:6227–38.
 Park G, Yim S, Yoon Y, Kim C, Seo D, Koichi E. Hydrogen production with
integrated micro channel fuel processor using methanol for portable fuel cell
systems. Catalysis Today 2005;110:108–13.
 Hsueh C, Chu H, Yan W, Leu G, Tsai J. Three dimensional analysis of a plate
methanol steam micro reformer and a methanol catalytic combustor with
different ﬂow channel designs. International Journal of Hydrogen Energy
 Telotte J, Kern J, Palanki S. Miniaturized methanol reformer for fuel cell
powered mobile applications. International Journal of Chemical Reactor
 Hsueh C, Chua H, Yan W, Chen C. Transport phenomena and performance of a
plate methanol steam micro-reformer with serpentine ﬂow ﬁeld design.
Applied Energy 2010;87:3137–47.
 Besser R. Thermal integration of a cylindrically symmetric methanol fuel
processor for portable fuel cell power international. International Journal of
Hydrogen Energy 2011;36:276–83.
 Bentley, JM, Mitchell, W, Clawson, L, Cross, J. US6783742B2; Aug. 31, 2004.
 Irving, P, Ming, Q, Harrison, J. DOE Hydrogen Program, 32 (FY2004 progress
 Sá S, Sousa J, Mendes A. Steam reforming of methanol over CuO/ZnO/Al2O3
catalyst. Part 1: Kinetic, modeling. Chemical Engineering Science 2011;20:
 Avgouropoulos G, Ioannides T, Kallitsis J, Neophytides S. Development of an
internal reforming alcohol fuel cell: concept, challenges and opportunities.
Chemical Engineering Journal 2011;176:95–101.
 Avgouropoulos G, Neophytides S. Performance of internal reforming metha-
nol fuel cell under various methanol/water concentrations. Journal of Applied
A. Iulianelli et al. / Renewable and Sustainable Energy Reviews 29 (2014) 355–368